porous electrode review
Post on 08-Jan-2016
Embed Size (px)
DESCRIPTIONPorous Electrode Review
147. -., Concentrated Polymer 5olutions: Part 111. Nor- mal Stresses in Simple Shear Flow, ibid., 13, 955 ( 1967b ) .
148. -., Correlation of Stress Data in Viscoelastic Poly- mer Solutions, ibid., 14,360 ( 1968).
149. Yamakawa, H., Transport Properties of Polymer Chains in Dilute Solution: Hydrodynamic Interaction, J . Chem. Phys., 53,436 ( 1970).
150. Yamakawa, H., Modern Theory of Dilute Polymer Soh- tions, Harper and Row, New York ( 1971 ).
151. Zimm, B. H. Dynamics of Polymer Molecules in Dilute Solution: Viscoelasticity, Flow Birefringence and Dielec- tric Loss, J. Chem. Phys., 24, 256 ( 1956).
152. - ., Theory of the Non-Newtonian Viscosity of High Polymer Solutions, Ann. N . Y . Acad. Sci., 89, 670 ( 1961).
153. -., and R. W. Kilb, Dynamics of Branched Poly- mer Molecules in Dilute Solution, J. Polymer Sci., 37, 19 (1959).
154. Zimm, B. H., G. M. Roe, and L. F. Epstein, Solution of a Characteristic Value Problem from the Theory of Chain Molecules, J . Chem. Phys., 24, 279 ( 1956).
155. Zimmerman, R. D., and M. C. Williams, Evaluation of Internal Viscosity Models, Trans. SOC. Rheol., 17, 23 (1973).
156. Zwanzig, R., Theoretical Basis for the Rouse-Zimm Model in Polymer Solution Dynamics, J . Chem. Phys., 60,2717 (1974).
157. - ., J. Kiefer, and G. H. Weiss, On the Validity of the Kirkwood-Riseman Theory, Proc. Nat. Acad. Sci., 60,381 (1968).
Mike Williams, born and bred in Wisconsin, took the con- venient but fortunate educational route through Madison. The B.S. led to a summer job at Los Alamos which stimulated his interest in rheology, and he returned to Madison to study con- tinuum modeling with Bob Bird. After getting his Ph.D. in 1964, Mike spent a year at the University of Oregon with Marshall Fixman and focused on molecular rheology. Since arriving at Berkeley, he has tied to synthesize these two re- search interests and has also dabbled in drag reduction, block copolymer thermodynamics, and flow-induced blood damage.
His extracurricular activities include a ridiculous degree of participation in baseball and tennis and a fannish interest in all sports, but most of his outside time is engaged in career guidance work with high school students.
Porous-Electrode Theory with Battery Applications
JOHN NEWMAN Lawrence Berkeley Laboratory and
Department of Chemical Engineering University of California
Berkeley, California 94720 Developments in the theory of flooded porous electrodes are reviewed
with regard to simulation of primary and secondary batteries, adsorption of ions and double-layer charging, and flow-through electrochemical re- actors. and
WILLIAM TIEDEMANN Corporate Applied Research Group
Globe-Union, Ins., Mihvaukee, Wisconsin
Porous electrodes have numerous industrial applications primarily because they promote intimate contact of the electrode material with the solution and possibly a gaseous phase. Specific factors are as follows:
1. The intrinsic rate of the heterogeneous electrochemi- cal reaction may be slow. A porous electrode can compen- sate for this by providing a large interfacial area per unit volume (for example, lo4 cm-1).
2. Double-layer adsorption constitutes the basis for novel separation processes involving cycling of the elec- trode potential. Just as in conventional fluid-solid adsorp- tion, a high specific interfacial area is desirable.
3. Important reactants may be stored in the solution in close proximity to the electrode surface by means of porous electrodes. This permits sustained high-rate discharge of the lead-acid cell. 4. A dilute contaminant can be removed effectively with
a flow-through porous electrode. The proximity of the flow- ing stream to the electrode surface is again important.
5. Similar arguments apply to nonconducting reactants of low solubility. Then another solid phase (as in batteries) or a gas phase (as in fuel cells) may be incorporated into
the system, or the reactants may be dissolved and forced through a porous electrode.
6. The compactness of porous electrodes can reduce the ohmic potential drop by reducing the distance through which current must flow. This has obvious advantages in reducing the losses in batteries and fuel cells. It may also permit operation without side reactions by providing po- tential control for the desired process.
If porous electrodes were trivially different from plane electrodes, there would be no motivation for their separate study. But here inherent complications arise because of the intimate contact of electrode and solution-the ohmic potential drop and the mass transfer occur both in series and in parallel with the electrode processes, with no way to separate them. One needs to develop an intuitive feeling for how and why the electrode processes occur nonuni- formly through the depth of the electrode. Finally, we seek methods for designing a porous electrode for a par- ticular application in such a way as to maximize the effi- ciency.
Electrodes with two fluid phases are excluded from con- sideration here. Gas electrodes for fuel cells are reviewed
AlChE Journal (Vol. 21, No. 1) January, 1975 Page 25
by Chizmadzhev et al. (1971) and by Bockris and Srini- vasan (1969) among others. The present article is also more concerned with macroscopic porous-electrode theory than with the detailed morphology and reaction mecha- nisms of particular chemical systems (see, for example, Burbank et al., 1971; Milner and Thomas, 1967) or with the growth of crystals or layers of insoluble products (see Hoar, 1959; Young, 1961; Vermilyea, 1963).
With these exclusions, a broad subject area remains. Battery electrodes illustrate an industrially important ap- plication of porous-electrode theory. Flow-through porous electrodes have some promise for recovery and removal of electropositive metals (Ag, Au, Cu, Hg, Pb) from dilute solutions, for electro-organic synthesis, and for oxidation of unwanted organic pollutants and surfactants. Transient double-layer charging and adsorption are of interest in the determination of the internal area of porous electrodes, in some separation processes, and in the interpretation of im- pedance measurements on porous electrodes.
Fundamentals of electrochemical thermodynamics, kinet- ics, and transport processes are not explained at length. We build here on earlier expositions of these subjects (see, for example, Newman, 1967, 1973).
The earlier reviews of Grens and Tobias (1964), Posey (1964), and de Levie ( 1967) are relevant and have been consulted particularly in regard to the early Russian litera- ture. See also Gurevich et al. (1974).
MACROSCOPIC DESCRIPTION OF POROUS ELECTRODES Porous electrodes consist of porous matrices of a single
reactive electronic conductor or mixtures of solids which include essentially nonconducting, reactive materials in addition to electronic conductors. An electrolytic solution penetrates the void spaces of the porous matrix. At a given cime, there may be a large range of reaction rates within the pores. The distribution of these rates will depend on physical structure, conductivity of the matrix and of the electrolyte, and on parameters characterizing the electrode processes themselves.
In order to perform a theoretical analysis of such a com- plex problem, it is necessary to establish a model which accounts for the essential features of an actual electrode without going into exact geometric detail. Furthermore, the model should be described by parameters which can be obtained by suitably simple physical measurements. For example, a porous material of arbitrary, random struc- ture can be characterized by its porosity, average surface area per unit volume, volume-average resistivity, etc. Simi- larly, one can use a volume-average resistivity to describe the electrolytic phase in the voids. A suitable model would involve averages of various variables over a region of the electrode small with respect to the overall dimensions but large compared to the pore structure. In such a model, rates of reactions and double-layer charging in the pores will have to be defined in terms of transferred current per unit volume.
A number of early and recent models represent the structure with straight pores, perpendicular to the external face of the electrode, and a one-dimensional approximation is introduced and justified on the basis of the small diame- ter of the pore compared to its length. As de Levie (1967) has pointed out, the mathematical equations to treat are essentially identical with those of the macroscopic model although a parameter such as the diffusion coefficient has a different interpretation. We shall prefer to speak in terms of the macroscopic model. The model set forth by New- man and Tobias (1962) has elements which can be found in the earlier work of Coleman (1946), Daniel-Bek (1948), Ksenzhek and Stender (1956a, b) , and Euler and
Nonnenmacher ( 1960). Refinements (Posey and Moro- zumi, 1966; Johnson and Newman, 1971, for example) permit the treatment of double-layer charging and make clearer the applicability to flow-through electrodes and electrodes with time-dependen t structural parameters. Average Quantities
In this macroscopic treatment, we disregard the actual geometric detail of the pores. Thus, we can define a poten- tial in the solid, conducting matrix material and another potential @z in the pore-filling electrolyte. These quantities, and others to be defined shortly, are assumed to be con- tinuous functions of time and space coordinates. In effect, the electrode is treated as the superposition of two con- tinua, one representing the solution and the other repre- senting the matrix. In the model, both are presen